706 T Maiyalagan, B Viswanathan and U V Varadaraju2. Experimental 2.3 Characterization methods2.1 Materials The scanning electron micrographs were obtained after the removal of alumina template using a JEOL JSM-840All the chemicals used were of analytical grade. Titanium model, working at 15 keV. For transmission electron micro-isopropoxide (Aldrich), 2-propanol (Merck) and Degussa scopic studies, the nanotubes dispersed in ethanol wereP-25 titanium dioxide (Germany) were used as received placed on the copper grid and the images were obtained(BET surface area, 50 m2/g and anatase : rutile ratio, 80 : 20). using Phillips 420 model, operating at 120 keV. The UV-Anodisc alumina membranes with a pore size of 200 nm vis absorption spectra were obtained on a Cary 5E spec-and thickness of 60 µm were purchased from Whatman trophotometer. The X-ray diffraction patterns were obtai-(catalog no. 6809-6022; Maidstone, UK). ned on a Philips PW 1820 diffractometer with CuKα (1⋅54178 Å) radiation. Micro-Raman scattering experi-2.2 Synthesis of TiO2 nanotubes ments were performed on a Bruker FRA106 FT-Raman at room temperature in a quasi-backscattering geometryTitanium isopropoxide (5 ml) was added to 25 ml of 2- with parallel polarization incident light. The excitationpropanol (mole ratio [Ti4+]/[2-propanol] = 1 : 20). The source used was an Argon ion laser operating at 514⋅5 nmsolution was stirred for 3 h at room temperature (298 K). with an output power of 20 mW.The alumina template membrane was dipped into thissolution for 2 min. After removal from the solution, vacuumwas applied to the bottom of the membrane until the entire 3. Results and discussionvolume of the solution was pulled through the membrane.The membrane was then air-dried for 60 min at 303 K The scanning electron microscopic (SEM) image of theand then placed in a furnace (in air) with a temperature TiO2 nanotubes obtained after dissolving the 200 nm alu-ramp of 2°C min –1 to 873 K for 2 h. The temperature was mina template membranes is shown in figure 1a. It can bethen decreased at a ramp rate of 2°C min –1 to room tem- seen that an ordered array of nanotubes with uniformperature (303 K). The ordered TiO2 nanotube arrays were diameter and length is formed. The individual TiO2 nano-obtained by dissolving the alumina template in 3 M aqueous tubes were characterized by TEM after dissolving theNaOH for several minutes. TiO2 nanotubes thus formed alumina membrane template. The open end and the hollowwere then washed several times with distilled water to nature of the TiO2 nanotubes have also been confirmedremove the dissolved anodic alumina membrane and re- by transmission electron microscopic (TEM) image asmaining NaOH solution. shown in figure 1b. The TEM image shows that the single Figure 1. SEM image (a) and TEM image (b) of TiO2 nanotubes obtained by sol–gel method calcined at 650°C for 2 h.
Fabrication and characterization of uniform TiO2 nanotube arrays 707TiO2 nanotube is straight and dense. The outer diameter the valence band (VB) to the conduction band (CB). Anof the nanotube is ca. 200 nm, retaining the size and near absorbance below 370 nm was observed for the TiO2cylindrical shape of the pores of the aluminium oxide nanotubes, which is ascribed to bulk anatase TiO2 . Heremembrane. This indicates that the diameter of the nano- the blue shift of absorption maximum with higher bandtube synthesized is controlled by the pore size of aluminium energy of TiO2 nanotubes compared with that of the bulkoxide membrane. This result is in agreement with other Degussa TiO2 can be attributed to the quantum-size effectreports on the sol–gel based template method (Lee et al (Takagahara and Takeda 1992).2004). The powder XRD was used to investigate the phase of Figure 2 shows the UV-vis absorption spectrum of the TiO2 nanotubes. The X-ray pattern of the TiO2 nanotubeanatase TiO2 nanotube compared with that of the Degussa arrays is shown in figure 3(b). The diffraction peaks ofTiO2 . The spectral lines for both TiO2 nanotubes and De- (101), (004), (200), (105) and (211) correspond to thegussa TiO2 exhibit only one characteristic absorption anatase TiO2 phase. The peak positions and their relativeband, which is assigned to the intrinsic transition from intensities are consistent with the standard powder diffrac- tion pattern of anatase-TiO2 and there is no preferred ori- entation. Figure 3 shows that the crystal phase of TiO2 nanotubes is polycrystalline anatase structure whereas the Degussa P-25 contains a mixture of anatase and rutile phases. Further, no peaks for the amorphous alumina membrane were observed in the TiO 2 nanotubes. The Raman spectra of fabricated anatase TiO2 nano- tubes and Degussa TiO2 are shown in figure 4. The result of XRD analysis is supported by the Raman spectra of TiO2 nanotubes as shown in figure 4(b). The vibration mode symmetries of the anatase are indicated. Raman peaks at 156⋅9, 206, 408⋅48, 529⋅54, 649⋅54 and 801 cm–1 were assigned to E g, E g, B 1g, A 1g, E g and B 1g, respectively. The positions and intensities of the six Raman active modes correspond well with the anatase phase of TiO2 (Bersani and Lottici 1998; Lei et al 2001). A weak overtone scattering (B 1g) at 801 cm –1 was observed in this study. Overtone can be found in both bulk Degussa TiO2 and nanotube, but the intensity of overtone is very less in bulk Degussa TiO2 . This is due to the large intensity ratio ofFigure 2. UV-vis absorption spectrum of (a) Degussa TiO2and (b) anatase TiO2 nanotube.Figure 3. X-ray diffraction patterns of (a) Degussa TiO2 as a Figure 4. Raman spectrum of (a) Degussa TiO2 and (b) fabri-reference and (b) TiO2 nanotubes obtained by sol–gel method cated anatase-TiO2 nanotube (The vibration mode symmetriescalcined at 650°C for 2 h anatase phase. of the anatase are indicated).
708 T Maiyalagan, B Viswanathan and U V Varadarajufundamental peak to overtone one makes it difficult to be Gratzel M 2001 Nature 414 338observed. While for nanotube, the decreasing ratio makes Gong D, Grimes C A, Varghese O K, Hu W, Singh R S, Chen Zit easy to be observed. No significant broadening and and Dickey E C 2001 J. Mater. Res. 16 3331shift of Raman spectra were found when one compared Hagfeldt A and Gratzel M 1995 Chem. Rev. 95 49 Homyara H et al 2001 Thin Solid Films 386 173the obtained anatase-TiO2 nanotube with that of the bulk Huang S Y, Kavan L, Gratzel M and Exnar I 1995 J. Electro-Degussa TiO2 . chem. Soc. 142 142 Kasuga T, Hiramatsu M, Hoson A, Sekino T and Niihara K4. Conclusions 1998 Langmuir 14 3160 Kavan L, Attia A, Lenzmann F, Elder S H and Gratzel M 2000 J. Electrochem. Soc. 147 2897In summary, highly ordered TiO2 nanotubes and nano- Lakshmi B B, Patrissi C J and Martin C R 1997 Chem. Mater. 9fibrils have been synthesized by sol–gel chemical method 2544within the pores of anodic alumina template membrane. Lee S, Jeon C and Park Y 2004 Chem. Mater. 16 4292The results of SEM and TEM show that the synthesized Lei Y, Zhang L D and Fan J C 2001 Chem. Phys. Lett. 338nanotubes have a uniform length, diameter and form a 231highly ordered array and the XRD measurements confirm Livraghi S, Votta A, Paganini M C and Giamello E 2005 Chem.the presence of polycrystalline anatase phase in the TiO2 Commun. 4 498nanotubes. This method can be employed for obtaining Macak J M, Tsuchiya H and Schmuki P 2005 Angew. Chem.large surface area TiO2 for use in photocatalysis and as Int. Ed. 44 2100electrodes in solar cells. Maiyalagan T and Viswanathan B 2005 Mater. Chem. Phys. 93 291 Martin C R 1996 Chem. Mater. 8 1739Acknowledgements Martin C R, Parthasarathy R and Menon V 1993 Synth. Met. 55 1165We thank the Council of Scientific and Industrial Research Poulios I, Kositzi M and Kouras A 1998 J. Photochem. Photo-(CSIR), India, for a senior research fellowship to one of biol. A: Chem. 115 175the authors (TM). Quan X, Yang S, Ruan X and Zhao H 2005 Environ. Sci. Tech- nol. 39 3770 Sander M S, Cote M J, Gu W, Kile B M and Tripp C P 2004References Adv. Mater. 16 2052 Takagahara T and Takeda K 1992 Phys. Rev. B46 15578Adachi M, Murata Y and Yoshikawa S 2000 Chem. Lett. 8 942 Uchida S, Chiba R, Tomiha M, Masaki N and Shirai M 2002Adachi M, Okada I, Ngamsinlapasathian S, Murata Y and Electrochemistry 70 418 Yoshikawa S 2002 Electrochemistry 70 449 Varghese O K, Gong D W, Paulose M, Ong K G, Dickey E CBersani D and Lottici P P 1998 Appl. Phys. Lett. 72 73 and Grimes C A 2003 Adv. Mater. 15 624Du G H, Chen Q, Che R C, Yuan Z Y and Peng L M 2001 Appl. Zhou Y, Cao L, Zhang F, He B and Li H 2003 J. Electrochem. Phys. Lett. 79 3702 Soc. 150 A1246